‘,9: . u-. . -
, .-. .a: i.~z"<&-. -. -
. . aw;
Similarities and differences of exemptions from PWHT for
C-Mn and low-alloy steels in several current codes are
reviewed, and some rationalizations are considered
BY D. J. ABSON, Y. TKACH, I. HADLEY,
V. S. WRIGHT, AND F. M. BURDEKIN
- , -his article compares and contrasts the current rules and
N guidelines present in various fabrication standards (mainly
U. S. and UK) regarding the postweld heat treatment
(PWHT) requirements of welds and the limits for as-welded con-
struction made in pipes, pressure vessels, and structures, including
bridges, buildings, and offshore structures, as discussed below. It is
recognized that some codes now include provision for repair with-
out PWHT (Refs. 1-3), and that there have also been investiga-
tions aimed at providing recommendations for acceptable thick-
ness limits for the as-welded condition for general structural con-
ditions (Refs. 4, 5). It is noted that steel making technology has
changed over the last thirty years or so (although steels are also
produced in parts of the world where steel making technology lags
behind best practice). However, the fabrication codes were gener-
ally devised for older, normalized steels with higher carbon con-
tents (Refs. 6, 7), and often with no toughness requirement.
In addition, a number of methods available for gaining ex-
emption from PWHT are examined, including specially designed
weld repair procedures and a case-specific fracture mechanics
approach (in Part2). The generalmethod adopted is that of Ref.
8, for which fracture mechanics testing, e. g., as in Ref. 9, is nor-
mally required. This investigation relates only to C-, C-Mn, and
low-alloy steels. Some of the similarities and differences are con-
sidered, and testing required to move toward elimination of the
apparent anomalies is considered. In compiling this article, the
views of representatives of fabricators and end users have been
The objectives of the study were to identify the types of ma-
terials where industry considers that there are grounds for seek-
ing wider exemption from PWHT; to compare and contrast the
limiting thickness requirements above which PWHT is required
and the associated Charpy test requirements for the as-welded
condition in standards relevant to the fabrication industry; to in-
vestigate the methods available for gaining exemption from
PWHT, namely the use of specially designed repair procedures
and the specification of a minimum Charpy energy, calculated
by a fracture mechanics approach; and to identify whether a fu-
ture program of toughness testing and residual stress measure-
ments on specific steels is needed to demonstrate a case for ex-
emption from PWHT.
D. J. ABSON and I. }MDLEYare with TWI, Granta Park, Great/ lbington, Cambridge, UK Y TKA CH, formerly with TWI, is now with Corus Swinden
Technical Center, Moorgate, Rotherham, UK. WRIGHT is a consultant‘, recently retired; formerly general manager IRD, Rolls-Royce. E M. BURDEKIN
was formerly professor at University of Manchester Institute of Technology.
WELDING JOURNAL 63
Table 1 — Limiting Thickness for which Postweld Heat Ireatment ls Not Required for C-Mn Steels According to Various Standards
a ASME Pl ASME P3 ASME P4 ASME P5 Comments
1 Group 1/C-Mn, Groups 1 and 2, Groups 1 and 2. Group 1. and
‘ Code and BS EN Group 1 and BS EN Group 1.4 and BS EN Group 5.1 BS EN Group 5.2
K ASME 32 mm increase to 16 mm, 93°C 16 mm, 121°C 16 mm, 149°C 2 27} at 20°C Toughness requirement increases
VIII (14) 38 mm with 93°C preheat, C$0.25% preheat, C$[).15% preheat, C$0.‘. l5% for 32 mm and as strength increases; allowable
preheat Re $448MPzt thickness increases as toughness
(2 20.1 at 20°C for increases and as strength
2 34 mm and Re decreases.
ASME 19 mm 16 mm, 95°C 13 mm, 120°C 13 mm, 150°C No explicit Charpy test requirement in the standard.
B31.1 (15) preheat, preheat, preheat,
C$0.25% C$0.l5% C$0.15%
ASME 19 mm 19 mm 13 mm, 149°C 13 mm, 177°C Rc$448MPa, C, ,2 18] Room temperature
B313 (16) preheat preheat, C$0.15% R, $517MPa, CV2 20.1 Charpy toughness
Re<656MPa, C, ,2 271 requirement for carbon-
and low alloy steels:
ASME 32 mm No explicit Charpy test requirement in the standard.
API 650 32 mm increase Gp I-I11 & 111A (defined in the standard)
(18) to 38 mm with C, 2 20J. Gp 1V-VI C, 2 41J; Gp VIA, CV2 48] if
90°C preheat Q & T or TMCP
API 620 32 mm, increase PWHT required for nozzles and attachments when wall
1 (19) to 38 mm with I thickness exceeded.
C. ,2 341 (2 401 for Test temperature $ (design
it Q&T grades) metal temperature —17°C).
K7 ' r C, , 2 34] For design metal temperature
> —40"C, if tested at or
i below this temperature
‘ C, , 2 401 Acceptable for design metal
' C, , 2 271 (2 34J Test temperature of —196°C
3 i in longitudinal ' for liquefied hydrocarbon gasses.
1 direction) . i
1 - AWS D1/1 ‘ - ' Limits set by contract drawings or specifications.
(29) i .
JIS B.8243 32 mm, increase - 16 mm, C$0.25% Tubing 16 mm, ‘ Tubing 16 mm, Rm <490MPa, CV2 20] _ At T $ minimum
(20) to 38 mm with I 95°C preheat C $0.15, 120° C $0.15, Cr $3.0, Rm 2 490MPa, CV2 27] operating temperature.
95°C preheat preheat; , 120“C preheat; . 120°C preheat; . ' ' ‘
' - ' PWHT all PW1-1_T all thick-
thicknesses of vesel nesses of vessel ‘
Stoom- 32 mm, ~ Fine-grained steel: C $0.23 and CE $0.55 and RC
we2en(21) C$0.23%, may $370 MPa and KV (perpendicular) 2 311 at 0°C and
increase to 40 mm also KV (parallel) 2 271 at -50°C and 32 mm
<t$40 mm and weld metal KV (perpendicular) 2 31J
at 0°C, and'as long as there is no accumulation
of weldments or extensive local stiffening, and a
hydrotest is carried out.
Fine-grained steel; C$0.23 and CE $0.55 and
Re $450MPa and t$32 mm, and as long
as there is no accumulation of weldments
or extensive local stiffening, there is
no toughness requirement.
I 3 Review of Current Practice and Code Requirements emption from PWHT. These studies showed there was still some
J. ‘ variation between codes. The results are included in Table 1,
Fabrication Standards for C-Mn Steel Pressure Vessels, Piping, where the requirements of the U. S. codes relate to ASME P1 to
i and Offshore Structures P5 steels. The table has been extended to include requirements
‘ for Charpy test properties, and to cover a range of other codes
survey was carried out in 1971 (Ref. 10) that showed that and standards.
‘ the requirements of various codes, in terms of the mate everal of the codes have a similar thickness limit, at ~32
, _ (rial thickness above which PWHT was required, varied , mm, above which PWHT is required. Provision is made in
} considerably. Later work in 1980 (Ref. 11) showed that, while Jiseveral codes (Refs. 14, 18-20, 25) to extend this limit to
considerable harmonization had taken place, significant diver- 38 or 40 mm if certain conditions, generally the imposition of a
genee remained. More recent work by Mohr (Ref. 12) and also preheat of the order of 93°C (200°F), are met. The notable ex-
by Salkin (Ref. 13), who reviewed the differences in thickness ceptions are ASME B31.1 (Ref. 15) and B313 (Ref. 16), with a
limits, in temperature ranges, and in hold times covering a range thickness limit of 19 mm, and EEMUA 158 (Ref. 28) that speci-
of steel types, has highlighted the limits and provisions for ex- fies a limit of 40 mm for nodes, with a limit of50 mm applying
Tllble 1 — Continued
Groups 1 and 2,
Groups 1 and 2,
Group 1, and
Code and BS EN Group 1 and BS EN Group 1.4 and BS EN Group 5.1 BS EN Group 5.2
:38 )2971 35 mm No Charpy test requirement.
BS 1113 30 mm, increase 13 mm, increase 513 mm thick 513 mm thick and C, >401
(23) to 35 mm with to 35 mm with and $127 mm 5127 mm diameter,
100°C preheat, 100°C preheat, diameter. Cs0.15%
C5025”/ a Cs0,25% Cs0.15%
BS EN <35 mm <13 mm <13 mm C, 2 271 for transverse Tm, S lowest scheduled
12952 (24) specimens (preferred) operating temperature
or c,2 351 ('rc, ,.2o“c).
BS 2633 30 mm, increase to 512.5 mm thick 512.5 mm thick $12.5 mm thick No Charpy test required.
(25) 35 mm 100°C and 5127 mm and 5127 mm and 5127 mm
preheat, CSO.25% diameter diameter, 120°C diameter, 150°C
preheat preheat, CsO.15%
PD 5500 35 mm, increase 12.5 mm, increase PWHT required PW1-IT required
(26) to 40 mm if CV‘ 2 271 to 19 mm with for all thicknesses for all thicknesses
at —20°C 100°C preheat
PD 5500 40 mm, but see R, <450MPa, c, z 27.1 Tm, = 2.94 (MDMT-10)°C
(Service R,2 450MPa, C. ,2 401 (PD 5500 Annex D)
PrEN 35 mm 515 mm thick, or 515 mm thick, or C2 27.1 or C. ,2 401 Test temperature depends
13445 (27) 513 mm thick and S13 mm thick and on strength, toughness
5120 mm diameter S120 mm diameter level, and design reference
and design temperature temperature.
EEMUA Minimum design R62 275 MP3, CV2 271 C, at —40°C, for assumed
158 (28) throat thickness: R52 355MPa, C, ,2 361 MDMT : -10°C.
-40 mm nodes 50 R62 450MPa, C, ,2 451
mm plain regions
BS 5950 t = k.50. 355 1-4. 1.2 MDMT-T271
max (F) ( ) ( 10 ) C, , required at MDMT, k = 2 for as-welded joints but
reduces with stress concentrations preent. '
to other regions. The apparent harmony is, however, in part illu-
sory, because the steels employed in the United States and the
United Kingdom are generally different in chemical composi-
tion (an issue that is considered in more detail later), and may
well have different inherent Charpy test properties.
It should be noted that the basic requirements of BS 1113
(Ref. 23) and BS 2633 (Ref. 25), which are shown in Table 1, re-
late to steels with sO.25%C, and those of Stoomwezen (Ref. 21)
to steels with sO.23%C; in these standards, PWHT is required
for steels with higher carbon contents. In BS 2633 (Ref. 25),
PWHT is not required for steels 535 mm thick if the service tem-
perature is above 0°C, while PD 5500 (Ref. 26) has the same re-
quirement for steels up to 40 mm thick. In Pr EN 13445 (Ref.
27), PWHT is only necessary in special cases, for example in H28
service. In some of the British Standards (Refs. 22, 25, 26), PWHT
is required, even up the limiting thickness shown, if it is speci-
fied by the purchaser.
. he general trends revealed by the tabulation are for the
I' permitted thickness without PWHT to decrease with in-
I creasing alloy content of steels and/ or for increased pre-
heat to be required, together with reductions in maximum car-
bon level permitted. For low-alloy steels containing s1.5%Cr and
s0.5%Mo (including ASME P4 groups 1 and 2 steels), and also
for 2.25%Cr-1%Mo steels (including ASME P5 group 1 steels),
there is greater uniformity among the standards, and there are
some strong similarities between the BS 2633 requirements and
those of ASME VIII and ASME B31.1 and B31.3.
In Table 1, it will be noted that in ASME VIII (Ref. 14), API
650 (Ref. 18), BS 1113 (Ref. 23), and BS 2633 (Ref. 25), there is
a marginal increase in the thickness limit if a preheat at a mini-
mum temperature of ~93°C (200°F) is used. The reason for this
is not known, and has not been discovered in the contacts made
with representatives of the fabrication industry. It may reflect an
anticipated increase in toughness or avoidance of hard local brit-
tle zones from a slight reduction in as-welded HAZ hardness, as
well as a reduced likelihood of hydrogen-assisted fabrication
Fabrication Standards for Buildings and Bridges
The material thickness requirements for bridges and build-
ings, as specified in BS 5950: 2000 (Ref. 30) and BS 5400: 2000
Part3 (Ref. 31), have been examined. These specifications are
much less prescriptive regarding requirements for exemption
from PWHT; most welded connections in bridges and buildings,
including those in thick sections, are left in the as-welded condi-
tion, and the emphasis is on the use of materials with sufficient
fracture toughness not to require PWHT. Indeed, BS 5950 does
not consider PWHT at all. However, these codes do provide ma-
terial thickness limits. Unlike some of the pressure vessel and
piping codes examined previously, the limiting thickness require-
ments are dependent upon service temperature, yield strength,
and Charpy impact properties.
; summary of strength and impact values for current Eu-
Aropean structural steel products is given in Ref. 5. All the
_new European structural steel grades are supplied to a
minimum Charpy impact level. The minimum Charpy toughness
requirements are 27 1 at -50°C for most grades, with some re-
WELDlNG JOURNAL :
quirements being 40 J at —20°C (which is approximately equiva-
lent to 27 J at ~30°C). However, there may be a limiting thick-
ness up to which the impact toughness is guaranteed. For exam-
ple, in BS EN 10025 (Ref. 32), this limiting thickness for nonal-
loyed grades is 250 mm for plates and 100 mm for sections.
he limiting thickness values in BS 5950 (Ref. 30) and BS
I 5400 (Ref. 31) are presented as general equations; the
form of these equationsis the same for both specifica-
tions, although differences exist in calculating the so-called k-
The equations, the background to which is explained in more
detail in Ref. 5, are shown below.
T, ,,, .,, 2 T27, — 20 as 5950 and BS5400:
tS 50k 9-53 1.2 at ‘T271
Tm)" < T27] —
ts 50K 355 35 +Tmiri ‘T271 1.2 Tmin ‘T27!
cry 15 10
BS 5400: not permitted
where t is the maximum permitted thickness of the part under
stress in mm; k is the k-factor (see below); cry is the nominal yield
strength of the part; Tm, “ is the design minimum temperature of
the part in °C; T27} is the temperature in degrees Celsius for which
a minimum Charpy energy of 27 J is specified by the product stan-
dard for impact tests on longitudinal V-notch test pieces.
The k-factor is the product of four subfactors relating to sus-
ceptibility to brittle fracture, as follows:
k= kd-k -kc-ks
and takes values ranging from <0.25 to 4. Low values of k de-
note higher susceptibility to brittle fracture, e. g., high applied
stress, high strain rate, or the presence of stress concentrations.
The subfactors each account for a different aspect of susceptibil-
ity to brittle fracture, as follows:
° kd accounts for the weld detail, and takes values between
0.5 and 2, which can be increased by 50% if PWHT is applied.
' k accounts for the presence of gross stress concentrations
and tallies values up to 1.
° kc, takes account of stress levels, with values ranging from 1
° ks takes account of high strain rates, with values of 0.5 (for
areas likely to be loaded under impact) and 1 (for all other areas).
5 an example, the maximum permitted thickness of a
Agrade 355 steel in the as-welded condition, subjected to
Charpy testing at the material design minimum temper-
ature (MDMT), would be 50 mm for the condition k = 1, i. e.,
with simple weld details, quasi-static strain rates, and no gross
stress concentrations. This is broadly comparable with the upper
range of allowable thicknesses of Table 1. However, the limiting
thickness for the same as-welded joint could be as low as 14 mm
under the same applied stresses and strain rates, if gross stress
concentrations and poor weld details are present. If high-strain-
rate loading also applies, e. g., bridge parapets, it could be even
lower at 7 mm. Conversely, for simple welded joints under low
applied stress, the limiting thickness could be as high as 100 mm,
and even 150 mm if the fabrication is subjected to PWHT.
The fracture avoidance rules given in BS 5400 Part3 (Ref. 31)
are based on fracture mechanics calculations, calibrated against
other considerations such as the results of full-scale tests on sim-
66 MARCH 2006
The steels employed in the
United States and the
United Kingdom are generally
different in chemical composition,
and may well have different
inherent Charpy test properties.
ulated bridge details, and case histories of bridge failure. Details
of these calculation methods are described in Ref. 5.
Eurocode 3 —— Design of Steel Structures
The requirements of Eurocode 3 (Ref. 33) have also been ex-
amined. Note that the document examined is a draft for devel-
opment (DD ENV), and so is subject to change before final issue
as a Eurocode. The document contains a procedure based on
fracture mechanics principles and the Master Curve correlation
between fracture toughness and Charpy energy.
D jasically, the procedure determines the required fracture
toughness for a steel component, depending on factors
J" such as steel strength grade, section thickness, loading
speed, lowest service temperature, applied stress, application of
PWHT, type of structural element, and consequences of failure.
The provisions of the draft Eurocode (Ref. 33) are fairly sim-
ilar to those of BS 5400 (Ref. 31) (and therefore similar to the
upper range of Table 1) for the case k = 1, i. e., where there are
no gross stress concentrating features or fatigue-sensitive weld
details. However, whereas under BS 5400 the maximum permit-
ted thickness for the same as-welded joint under similar applied
stress and at a similar strain rate could range from 14 to 50 mm,
it would remain 50 mm throughout under the draft Eurocode.
The draft Eurocode (Ref. 33) and BS 5400-3 (Ref. 31) re-
quirements are compared and contrasted in detail in Ref. 5, where
concern is expressed at some of the potentially unsafe provisions
of the former.
Review of Documentation for Low-Alloy Steels
rily from the United States and United Kingdom, have
“_, ,,_, .-also been reviewed. The information is also summarized
in Table 1. See Table 2 for the compositions of relevant ASME P
numbers. For such steels, there are some strong similarities in
the requirements relating to exemptions from PWHT between
the U. S. and UK codes. In Table 1, BS 2633 (Ref. 25) stipulates
a similar preheat to the U. S. codes. However, the requirements
of ASME B31.3 (Ref. 16) differ from the other codes in that
PWHT is not required for ASME P3 Grades 1 and 2 steels up to
19 mm thick, while this code requires a higher preheat for P4
Grades 1 and 2 and P5 Grade 1 steels. It should be recognized
that the situation is appreciably more complex than these num-
bers in Table 1 suggest, as different recommendations apply to
specific weldments. See, for example, the footnote to ASME VIII
Division 1 Table UCS-56 (Ref. 14), which includes clauses relat-
ing to nozzle connections, and the welding of pressure parts to
nonpressure parts. The additional requirement to gain exemp-
tion from PWHT for tubes less than or equal to 13-mm thickness
and less than or equal to 120-mm diameter in P5—type steels in
Pr EN 13445 (Ref. 27) is that the design temperature should ex-
Low—alloy steels in piping and pressure vessel codes, prima-
fable 2 — Summary of Information on Relevant ASME P Numbers
ASME P Number
Pl group 1
P3 groups 1 and 2
F4 groups 1 and 2
P5 group 1
Differences between Material Grouping Systems in
the ASME, CEN, and British Standard Codes
The grouping of materials used for welding has been carried
out under the auspices of the different code standards commit-
tees in both Europe, including the United Kingdom, and the
United States. In the United States, steels have been allocated a
P number or S number, but since 1998, materials used for welder
qualification may conform to other national or international stan-
dards or specifications, provided that the requirements for me-
chanical properties and specified analysis limits of the P or S
number are met. In the United Kingdom, materials have been
given group numbers in BS 4870 (Ref. 34) (for welding proce-
dures) and BS 4871 (Ref. 35) (for welder qualifications). Both of
these standards have been superseded by European standards
BS EN 288 (Ref. 36) and BS EN 287 (Ref. 37). A submission was
made to the committee compiling CR TR 15608, the draft guide-
lines for a metallic material grouping system (Ref. 38) by Sperko
(Ref. 39). In his proposed Annex to CR TR 15608, he attempted
to unify the ASME and CRTR 15608 grouping. He examined 985
relevant U. S. steel specifications and found the following:
1) 196 steel compositions could be classified within an ASME
2) Of the 196, only 91 C-Mn steels could be given a CR TR
15608 group number.
This study has indicated that, in terms of an ASME or CEN
grouping system, material grouping does not provide a basis for
exemption from PWHT. It would clearly be of considerable ben-
efit in moving toward more uniform PWHT requirements if steel
producers were to extend the practice of dual, or even multiple,
certification of steels, so that greater uniformity is achieved in
the compositions of steels. The practice would also facilitate the
eventual unification of standards.
separate codes for pressure vessels and piping, in terms
3: __of preheat and other requirements, have not been in-
cluded, Table 1 indicates that rationalization of the PWI-IT ex-
emption of all the codes would not be easy to achieve. For C-Mn
steels, a comparison of codes, in terms of maximum wall thick-
: lthough the fundamental details of the differences in the
ness where PWHT is not required and maximum carbon equiva- .
lent of material permitted, has suggested an even more widely
spread divergence. The codes are for different engineering appli-
cations. Differences between these may include different design
stress criteria, different inherent Charpy test requirements, and
(through the inspection codes) different allowable defect sizes.
The codes were drawn up by different professional bodies, based
on extensive experience and engineering practice. Therefore, dif-
ferences arose and inconsistent requirements ensued. The gross
differences that have arisen are likely to preclude the issue of a
unified code requirement giving exemption from PWHT.
Three of the main groups of steel users with an interest in ob-
taining exemption from PWHT are the petrochemical industry
through the Engineering Equipment and Materials Users Asso-
ciation (EEMUA) Material Technology Committee, the power
generation industry (through the Electricity Generators Welding
Panel (EGWP)) and the general structural industry. The data
covered in this review suggest that reconciliation of the require-
ments of these user groups may not be possible. It would clearly
be of benefit to the power generation industry to increase the
thickness threshold for PWHT, for example to the 40 mm em-
bodied in EEMUA 158 (Ref. 28) for C-Mn steels. Examination
of the data also raises questions about the need to give a PWHT
to weldments covered by BS 1113 (Ref. 23) and BS 2633 (Ref.
25) when the carbon content exceeds 0.25%. This limitation ap-
pears questionable, in the absence of such a condition in the other
codes, but should be considered in relation to the Charpy prop-
erties of the steels concerned.
C-Mn and Cr-Mo Steels
1 embodied in ASME 1331.1 (Ref. 15) and 1331.3 (Ref. 16),
,_ ; _ compared with the other standards, may reﬂect the likeli-
hood that the welding will be carried out in the field, and that
defect rates and defect sizes may be greater than for shop welds.
Girth welds in steel pipes have been subjected to a fracture me-
chanics assessment by Mohr (Ref. 40), who assumed the pres-
ence of root defects, and who concluded that the fracture resist-
ance of pipes thicker than 19 mm was at least equal to that of
thinner_ walled pipes. As PWHT is not required by ASME B31.1
for thinner walled pipes, presumably because the fracture resist-
ance has been found to be sufficient, Mohr questioned the need
for PWHT of thicker walled pipe if a fixed (rather than a pro-
portional) ﬂaw size is assumed in the calculations. However, all
of these considerations need to be seen in the context of the in-
herent Charpy properties of the materials concerned, and this is
not explicitly treated in some of the codes involved.
Tghe position of the general structural industry is that the
For C-Mn and Cr-Mo steels, the lower thickness threshold
scale and size of structures is so large that PWHT of the
V _ overall structure is impracticable, and PWHT is only con-
sidered for local sub-assemblies under exceptional circumstances.
Virtually all welded connections in bridges and buildings, includ-
ing those in thick sections, are left in the as-welded condition,
and the emphasis is on the use of materials with sufficient frac-
ture toughness not to require PWHT. Fracture mechanics calcu-
lations were used in defining the fracture avoidance rules given
in BS 5400 Part 3 (Ref. 31), and these were calibrated against
other information, including the results of full-scale tests on sim-
ulated bridge details, and case histories of bridge failure. The de-
tailed history of the piping codes is not known, but it is likely that
custom and practice made a greater contribution, no doubt with
some experience of failures incorporated. Also, it is noted that
ASME B31.1 (Ref. 15) and ASME B31.8 (Ref. 17) provide for
nonimpact tested steels to be used. However, since the code de-
velopment took place, steel-making technology has changed sig-
nificantly, steel toughness levels have generally improved sub-
stantially, and (at least within Europe) steel specifications com-
monly incorporate impact toughness requirements. It is, there-
fore, likely that limiting thicknesses could be increased, and thus
PWHT omitted, as was shown to be acceptable for the steel ves-
sels subjected to an ECA by Leggatt et al. (Ref. 41).
WELDING JOURNAL 57
In spite of the disparities between the PWHT requirements
of the pressure vessel and piping standards depicted in Table 1,
some rationalization could be effected by building on the simi-
larities that do exist. One possible approach would be to define
a modest limiting thickness, perhaps -32 mm, for which there
are few additional requirements and a minimum level of absorbed
Charpy energy could be assumed for the steels concerned. A
greater limiting thickness could then be accommodated if addi-
tional requirements were met. This is the approach adopted in
PD 5500 (Ref. 26), where the additional requirement is a mini-
mum Charpy impact toughness (of2 271 at —20°C) for the higher
level of limiting thickness of 40 mm. More extensive require-
ments for the same limiting thickness are imposed in Stoomwezen
(Ref. 21). These are C S0.23%, IIW CE £0.45, RC S370 N/ mmz,
both C, 2 27 J at —50°C and C, , 2 31 J at 0°C for the base steel,
and C, 2 31 J at 0°C for the weld metal. It will be noted that the
codes do not mention explicitly as-welded HAZ toughness, even
though this factor would probably be limiting if HAZ fracture
toughness were to be measured and a detailed engineering criti-
cal assessment were to be carried out.
— his present study has demonstrated that code classifica-
I‘ tions and material groupings do not provide avenues for
, _ a uniform approach across all the codes, at least for C and
C-Mn steels, for the omission of PWHT following welding. PD
5500:2000 (Ref. 26) provides an Appendix that can be used to
justify exemption from PWHT. The justification is based on a de-
sign reference temperature calculation. However, it appears that
this philosophy has been adopted only in this pressure vessel
code, and the approach may not gain wide acceptance in codes
for other applications. A material properties, rather than code-
based, approach might be more widely acceptable. What appears
to be required is a knowledge base of weldment impact value/ frac-
ture toughness properties for welds deposited with known weld-
ing parameters. It may then be possible for codes to include HAZ
toughness requirement for weldments.
1' without PWHT have been reviewed for C and C-Mn steels
. and some low-alloy steels, and the requirements of dif-
ferent codes have been compared. The conclusions are as
1) U. S. and UK code requirements are generally similar in
the limiting thickness of C and C-Mn steels (including ASME P1
steels) beyond which PWHT is required for pressure vessels, pip-
ing, and storage tanks, at ~32 mm. However, differences in the
chemical compositions of U. S. and UK steels influence PWHT
requirements. The major exceptions in this area are ASME B31.1
and B313 (limiting thickness 19 mm). However, general struc-
tural codes, such as BS 5400 for bridges, BS 5950 for buildings,
and EEMUA 158 for offshore structures, permit significantly
higher thicknesses in the as-welded condition, linked to increas-
ing Charpy energy requirements.
2) For low-alloy steels containing S1.5%Cr and S0.5%Mo (in-
cluding ASME P4 groups 1 and 2 steels), and also for 2.25%Cr-
1%Mo steels (including ASME P5 group 1 steels), there are some
strong similarities between the BS 2633 requirements and those
of ASME VIII and ASME B31.1 and B31.3. The general trends
are for the permitted thickness without PWHT to decrease with
increasing alloy content of steels and/ or for increased preheat to
be required, together with reductions in maximum carbon level
3) In view of the differences that exist in the chemical com-
positions of broadly comparable U. S. and UK steels and the lack
of consistent requirements for Charpy test properties (as far as
”‘r; ‘s*‘f MARCH 2006
c: ode requirements for permitting as-welded construction
ASME and CEN are concerned), alignment by material group-
ing for C-Mn steels is not universally possible as a basis for ex-
emption from PWHT‘.
4) Since the development of the earliest codes, steel-making
technology has changed significantly, steel toughness levels have
generally improved substantially, and (at least within Europe)
steel specifications commonly incorporate impact toughness re-
quirements. It is therefore likely that limiting thicknesses could
be increased, and thus PWHT omitted.
5) UK code requirements for general structures such as
bridges, buildings, and offshore structures permit significantly
greater thicknesses to be used in the as-welded condition, linked
to Charpy toughness requirements for different grades of steel,
based on fracture mechanics analyses. The requirements can be
expressed in terms of MDMT — T3” (the temperature difference
between the material design minimum temperature and the tem-
perature for 27 J energy absorption in the Charpy test) and the
yield strength of the steel, for given assumptions about ﬂaw size
and stress level.
I) Where the relevant fabrication codes require that a PWHT
be carried out, consideration should be given to carrying out a
fracture mechanics assessment, with the agreement of all inter-
ested parties, in order to extend the thickness beyond which
PWHT is required.
2) Typical Charpy test data should be reviewed and collated
in terms of thickness and material type and IIW CE for steels
. supplied against the various standards summarized in Table 1.
Following completion of the review, consideration should be
given to the following cases: C- and C-Mn steels that would po-
tentially allow an increase in the ASME B31.1 and B31.3 thresh-
old thickness level for PWHT, and C- and C-Mn steels with
<0.25%C, to establish if the BS 1113 and BS 2633 requirements
3) Consideration should be given to the generation of tough-
ness data for thicknesses >12.5 mm and where Charpy energy
requirements are not unduly onerous, to see where the avoid-
ance of PWHT can be justified.
4) Steel producers should be encouraged to extend the prac-
tice of dual, or even multiple, certification of steels, so that greater
uniformity is achieved in the compositions of steels, thereby fa-
cilitating the eventual unification of standards.
5) Consideration should be given to introducing HAZ tough-
ness requirements into fabrication codes.
Helpful discussions with C. S. Wiesner and other colleagues
at TWI, and input from D. J. Allen of Powergen, B. Parry-Mills
and M. Coleman of British Energy, and R. Carroll of Foster
Wheeler Energy Limited are gratefully acknowledged. The work
was carried out within the Core Research program of TWI, which
was funded by Industrial Members of TWI.
I. ASME Boiler and Pressure Vessel Code, Section III, 2004. Rules for
construction of nuclear facility components. American Society of Mechani-
cal Engineers, N. Y., paragraph NB-4622.9, Temper bead weld repair.
2. ASME Boiler and Pressure Vessel Code, Section XI. 2004. Rules for
service inspection of nuclear power plant components. American Society
of Mechanical Engineers, N. Y., paragraph IWA-4623.1 Temper bead
welding of similar materials — Shielded metal arc welding.
3. National Board Inspection Code —A Manual for Boiler and Pres-
sure Wssel Inspectors, 2004 National Board of Pressure Vessel Inspec-
tors, Columbus, Ohio.
4. Burdekin. F. M. 1981. Materials aspects of BS5400: Part (3, paper 4
in The Design ofSIec/ I3riclges. ELI. K. C. Rockcy and H. R, Evans, Granada
ISBN 0 2461 1339 l.
5. Ogle. M. 1-1., Burdekin, F. M. , and Hadley, I. 2003. Material selec-
tion requirements for civil structures. Proe. lIWInt. Conff on Welded Con-
struction for Urban Infrastructure, 56th Annual Assembly of the IIW,
Bucharest, Romania, Ed. D. Dehclcan, International Institute of Weld-
ing, pp. 201-229.
6. Spaeder, C. E. , and Dory, W. D. 1995. Report No. 2, ASME post-
weld heat treating practices: An interpretive report. Welding Research
Council Bulletin 407. pp. 50-65.
7. Hancock. P. . Chubb, J. P. , and Spurrier, J. 1995. A new perspective
on the influence of thickness and post—we| d heat treatment for large scale
weldedjoints. J Engineering Materials and Technology, pp. 117, 209-214.
8. BS 7910: 1999. Guide on Methods for/ Issessing the Acceptability of
Flaws in Metallic Structures, incorporating Amendment 1, now super-
seded by BS 7910: 2005: Guide on Methods forAssessing the Acceptability
of Flaws in Metallic Structures.
9. BS 7448: Part 2: I997. Fracture Mechanics 777uglzness Tests —— Method
for Determination ofKh, critical C TOD, and Critical] Values of Welds in
10. Nicholson, S. , and Brook, J. C. Review of codes. 1971. Proc. Bi-
ennial Con/ ". On Heat Treatment. Joint Committee Iron and Steel Inst. ,
11. Saunders, G. G. 1980. Residual stresses and their reduction. Devel-
opments in Pressure Vessel Technology—3, Applied Science Publishers Ltd.
12. Mohr, W. 1994. Post-weld heat treatment: A review. Inspection,
assessment and repair of welded structures and components. I0thAn-
nual North American Welding Research Conference, Columbus, Ohio.
13. Salkin, R. V 1988. The desirability of unifying ideas and codes on
stress relief thermal heat treatments. FWPJournal, Part 1 Nov. , pp. 27-34,
Part 2 Dec. , pp. 5-13.
14. ASME VIII Div. 1: 2004. Rules for Construction of Pressure Vessels.
15. ASME B31.1. 2004. ASME Code for Pressure Piping, Power Piping.
16. ASME B31.3. 2004. ASME Code for Pressure Piping, Process Piping.
17. ASME B31.8: 2003. ASME Code for Pressure Piping, Gas Trans-
mission and Distribution Piping Systems.
18. API 650. 1998. Welded steel tanks for oil storage.
19. API 620. 2002. Design and Construction ofLarge, Welded, Low-
Pressure Storage Tanks. American Petroleum Institute.
20. JIS B 8243. 1981. Construction of pressure vessels. Now super-
sede by JIS B 8265: 2003 and JIS B 8266: 2003.
21. Rulesfor Pressure Vessels. 1991. Vol. 2, Section W 0701. Heat treat-
ment of unalloyed and low alloy steel, and Section W 0702 Heat treat-
ment of unalloyed and low alloy steel pipes. Dienst voor het Stoomwezen,
The Hague, (updated 1998.)
22. BS 2971: 1991. Specification for Class II arc welding of carbon
steel pipework for carrying fluids. British Standards Institution, includ-
ing amendment 1, February 1998.
23. BS 1113: 1999. Design and Manufacture of Water-Tube Steam
Generating Plant (including superheaters, reheaters and steel tube
24. BS EN 12952: 2001. Water Tube Boilers and Auxiliary Installations,
Part 2 — Materials for pressure parts of boilers and accessories, and Part
5 — Workmanship and construction of pressure parts of the boiler.
25. BS 2633: 1987. Class I Arc Welding ofFerritic Steel Pipework for
26. British Standards Institution Published Document PD 5500, 2003.
Unﬁred Fusion Welded Pressure Vessels. i
27. BS EN 13445: 2002. Unﬁred Pressure Vessels, Part 4 -— Manufacture.
28. EEMUA 158: 2000. Construction Speciﬁcation for Fixed Offshore
Structures in the North Sea.
29. AWS D1.1/D 1.1M: 2002. Structural Welding Code — Steel. Miami,
FIa. : American Welding Society.
30. BS 5950-1: 2000. Structural Use ofSteelwork in Building. Code of
practice for design — Rolled and welded sections.
31. BS 5400-3: 2000 (incorporating Corrigendum 1). Steel, Concrete
and Composite l3I'l(lg‘. S', Part 3 ——- Code of practice for design of steel
32. BS EN 10025: 1993. Hot Rolled Products 0fNon-alloy Structural
Steels‘ — Tit: /I/ llL‘al Delivery Cotitlitions.
33. DD ENV 1993- 1-1:1992. Eurocode 3: Design ofSteel Structures,
Part 1.1—- General rules and rules for buildings.
34. BS 4870: 1981./ lpproval Testing of Welding Procedures, Part 1 —
Fusion welding ofsteel. (Superseded by BS EN 288-1: 1992, and BS EN
35. BS 4871: 1992. Approval Testing of Welders Working To Approved
Welding Procedures, Part 1 — Fusion welding of steel. (Superseded by BS
EN 287-1: 1992.)
36. BS EN 288: Part 1: I992. Speciﬁcation and Approval of Welding
Procedures for Metallic Materials — General Rules for Fusion Welding, and
BS EN 288: Part 3: 1992. Specification. and Approval of Welding Proce-
dures for Metallic Materials — Welding Procedure Tests for t/ ‘I8/Il‘C Welding
37. BS EN 287, Part 1: 1992. Approval Testing of Weldersfor Fusion
38. British Standards Institution, Published Document PD CR ISO
15608: 2000. Welding — Guidelinesfor :1 Metallic Material Grouping Sys-
39. Sperko, W. J. 1998. Assignation of ASME materials to the new
grouping system CR TR 15608, CEN/ TC 121/SC I N, p. 407.
40. Mohr, W. C. 1997. Fracture mechanics to justify the minimum
thickness for PWHT: Girth butt-welded steel pipe. Edison Welding In-
stitute Report for Research Members MR9708.
41. Leggatt, R. H. , Muhammed, A. , Smith, A. T. , and Cheaitani, M.
J. 1999. Using fracture mechanics to claim exemption from PWHT—
Four case studies. TWI Report for Research Members 679/1999.
INDUCTION HEATING CABLES
ELECTRIC ARC FURNACE CABLES
FUSION & PARTICLE RESEARCH CABLES
ROBOT DRESS-OUT COMPONENTS
COMPLETE ROBOT DRESS-OUT PACKAGES
CABLE PROTECTIVE COVERINGS
CUSTOM MOLDED SERVO CABLES
QUICK-DISCONNECT PRIMARY CABLES
CUSTOM CONTROL CABLES
ALL T0 DAY
WWW. FLEXCABLE. COM
Circle No. 36 on Reader Info-Card
WELDING JOURNAL 69